0 INTRODUCTION

To evaluate structural reliability of dynamically loaded components it is necessary to know the scatter of the loading spectra as well as the scatter of the fatigue-life durability curve of the structural material [1] to

[7]. Structures that are made from spring steels are
typically subjected to a large number of load cycles.
For this reason, a S-N fatigue-life curve is normally
used to predict the fatigue life of such structures. In
the past it was presumed that a fatigue-life limit *Sa;FL*
exists at a certain number of load-cycles-to-failure

*NFL*, e.g., for structural steels the fatigue-life limit
should occur between 2×106 _{[8]}_{ and 10}8 _{[9]}_{ }
load-cycles-to-failure, see Fig. 1. However, it turned out
that for most metallic structural materials there is no
fatigue-life limit [10]. What exists in practice is a
so-called Haibach’s knee point, below which the slope of
the S-N curve is reduced. This part of the S-N curve
is usually referred to as a very-high-cycle domain.
Haibach [11] proposed a model for the S-N curve in
which the slope below its knee-point is 2*k*–1, if its
slope in the high-cycle domain is *k*,see Fig. 1.

Additionally many other researchers have shown that the slope of the S-N curve in the very-high-cycle domain is reduced ([12] to [14]). What is common to all these cases is that, not only the slope, but also the scatter of the experimental fatigue-life data, is

significantly changed (i.e. increased) below the knee point of the S-N curve, see Fig. 2.

Fig. 1. A S-N fatigue-life curve

It was further shown [13] and [14] that the slope of the fatigue-life curve in the very-high-cycle domain is much smaller than the one proposed by Haibach. In order to make reliable predictions of the structure’s fatigue life in the high-cycle and very-high-cycle domains one must be able to model the variable trend as well as the variable scatter of the number of load-cycles-to-failure for these two domains of the S-N curve.

The shape of the S-N curve in the vast neighbourhood of the knee point between the high-cycle and very-high-high-cycle fatigue domains of the S-N

**An Improved Model for Predicting the Scattered S-N Curves**

Klemenc, J. – Podgornik, B.
Jernej Klemenc1,*_{ – Bojan Podgornik}2

1_{University of Ljubljana, Faculty of Mechanical Engineering, Slovenia }
2_{Institute of Metals and Technology, Slovenia}

*In this article an improved neural network model is presented that allows us to predict the scattered S-N curves. The model is capable of *
*predicting the S-N curve in its high-cycle and very-high-cycle fatigue domains by considering also the increased scatter of the fatigue-life *
*data below the knee point of the S-N curve. The scatter of the fatigue-life data for an arbitrary amplitude-stress level is modelled with a *
*two-parametric Weibull’s probability density function, the parameters of which are varied as a function of the amplitude-stress level. The *
*parameters of the S-N curve trend and its scatter distribution are not fixed, but depend on the parameters of the production process via a *
*serial-hybrid neural network. The article presents the theoretical background and the application in the case of real experimental fatigue data *
*for 51CrV4 spring steel manufactured with two different manufacturing technologies and two different heat treatments.*

Keywords: 51CrV4 steel, conventional manufacturing technology, electro-slag remelting, S-N curve, serial hybrid neural network Highlights

*• A model for predicting S-N curves and their scatter for 51CrV4 steel was built. *

*• The model is capable of predicting the S-N curves in the transition zone between high-cycle and very high-cycle fatigue *
*domains. *

curve is similar to the shape of the Coffin-Manson curve [15] in the neighbourhood of the transition between the low-cycle elastic-plastic domain and the high-cycle elastic domain of the fatigue-life curve. For this reason it is possible to model the S-N curve in the high-cycle and the very-high-cycle domains with a similar form:

*S _{a}*

_{= ⋅}

*a N*−

*b*

_{+ ⋅}

*c N*− +(

*b d*)

*a b c d*

_{>}

; , , , 0, (1)

where *Sa* represents the amplitude stress, *N* is the
number of load-cycles-to-failure and *a, b, c, d* are
parameters dependent on the material. We have shown
before [16] that it is possible to model the
fatigue-life curve of such a shape together with its scatter
by applying a Weibull’s two-parametric probability
density function (PDF) to describe the scatter of the
number of load-cycles-to-failure for an arbitrary
amplitude-stress level:

*N*→ *f N Sa* = ⋅ *N* *N*

⋅ −

−

( | ) β exp .

η η η

β 1 β

(2)

In that study we have presumed that the Weibull’s
scale parameter *η* (which represents the number
of load-cycles-to-failure at a 0.632 probability of

rupture) was dependent on the amplitude-strain level

*εa* via Coffin-Manson equation and that the Weibull’s
shape parameter *β* was constant [16]. However, there
is a huge difference between the scatter of the e-N
curve and the scatter around the knee point between
the high-cycle and very-high-cycle domains of the
S-N curve. While the width of the scatter band of the
e-N curve is constant below and above its knee point,
this is not the case for the knee point between the
high-cycle and very-high-high-cycle domains of the S-N curve.
In the latter case, the width of the scatter band of the
S-N curve in the very-high-cycle domain is much
larger than in the high-cycle domain, see Fig. 2. For
this reason it is not possible to describe the scatter of
such durability curve using a two-parametric Weibull
PDF from Eq. (2) with a constant shape parameter *β*.
On the contrary, to model the S-N curve around the
knee point between the high-cycle and
very-high-cycle fatigue domains the Weibull’s shape parameter

*β* should also depend on the amplitude-stress level *Sa*.
The objective was to build a model for predicting
the S-N curves and their scatter for a specific spring
steel. Since the material’s characteristics depend on
the manufacturing technology and the heat treatment
of such steels, these influential factors should be
considered when modelling the corresponding
S-N curves. The S-N curves can vary a great deal
between differently produced and/or heat-treated
steels, even for similar operating conditions. That
is why we decided to apply a serial hybrid neural
networks to build the model that is able to predict
the S-N curve and its scatter as a function of the
manufacturing technology and the heat treatment.
A similar approach was successfully applied before,
for modelling the dependence of the S-N and e-N
curves on the operating conditions ([17] and [18]). In
the scientific literature there exist a number of articles
on the application of neural networks for modelling
and predicting durability curves. However, most of
them are based on either multi-layer perceptrons or
basis functions. With such an approach it is difficult
to embed into a neural network an analytical model
that is capable for predicting trend and scatter of the
durability curve. Since the approach from Klemenc et
al. [18] was proved to be successful we modified it in
such a way that a new model is capable of predicting
the S-N curve in its high-cycle and very-high-cycle
fatigue domains by considering also the increased
scatter of the fatigue-life data below the knee point of
the S-N curve. The manufacturing technology and the
heat treatment were the inputs to the neural network
and the parameters of the S-N curve and its scatter
were its outputs.

Such a comprehensive model of the S-N curves with a capability of considering the increased scatter in the transition between the high-cycle and very-high-cycle domains has not been presented in the literature yet. A further innovation was to combine this model with the neural network in order to model the relationship between the parameters of the S-N curve and the applied manufacturing technology. The theory is explained in detail in section 1, experimental data are presented in section 2 and the results are presented and discussed in section 3.

1 THEORETICAL BACKGROUND 1.1 Variable-Scatter Model for the S-N Curve

To model the S-N curves and their scatter for a 51CrV4 spring steel a similar statistical model as used in [16]

was applied. Following this approach, the scatter of
the number of load-cycles-to-failure *N* for an arbitrary
amplitude-stress level *Sa* was described using a
two-parametric Weibull’s PDF, see Eq. (2) in section 1.
The trend of the S-N curve in the neighbourhood of
the knee-point was linked directly to the Weibull’s
scale parameter *η*:

*Sa* = ⋅*a* η(*Sa*)−*b*+ ⋅*c* η(*Sa*)− +(*b d*); *a b c d*, , , >0, (3)
with the Weibull’s shape parameter *β* that is now
dependent on the loading level *Sa*:

β β= = ⋅ +

+

### [

− ⋅ −### ]

≥ >

( )

exp ( ) ,

; , , .

*S* *f* *g*

*h S* *S*

*f* *g h S*

*a*

*a* *KP*

*KP*

1 1

1 0 (4)

With this equation the shape parameter *β* changes
continuously and smoothly from the value of *f* at
very low amplitude-stress levels to the value of
( *f·g*) at high amplitude-stress levels. The transition
gradient between the two limit values depends on the
parameter *h*, with the steepest gradient occurring at
the amplitude-stress value *SKP*. When combined with
the scale parameter *η* from Eq. (3) a small scatter
is obtained at high amplitude-stress levels and an
increased scatter is obtained at the lower
amplitude-stress levels that correspond to the very-high-cycle
fatigue domain.

To avoid illogical shape of the durability curves
around the knee point *Sa*= *SKP* two limit conditions are
defined:

1. The parameter *g* should never exceed the
following value of *glim*:

*g g* *b d*

*b*

≤ = +

⋅ −

lim max 3, .

5 1 (5)

2. The parameter *h* should never exceed the
following value of *hlim*:

*h h*

*b d*
*b*
*SKP* *f g*

≤ =

⋅ +

⋅

⋅ ⋅

lim

min ,

.

2 4

5

(6)

The two conditions in Eqs. (5) and (6) limit the
transition gradient between the small and large values
of the shape parameter *β* relative to the trend-curve
slope ratio (*b+d*)/*b*. The knee-point stress *SKP* is
calculated as a cross-section of the two asymptotes of
Eq. (3), see Fig. 2:

*SKP* = ⋅η*a* *KPb* , (7)

η_{KP}*a* *c*

*d*

= −

−

exp ln( ) ln( ) . (8)

In this way the S-N curve and its scatter in
the neighbourhood of the knee point between the
high-cycle and very-high-cycle fatigue domains is
modelled with seven parameters: *a*, *b*, *c*, *d*, *f*, *g* and *h*.
These parameters can be estimated using a numerical
optimisation process.

1.2 Serial Hybrid Multilayer Perceptron

Since the material characteristics of the spring steel
are dependent on the manufacturing technology
and the heat treatment, they are also reflected in the
trend and scatter of the corresponding S-N curve.
This means that the parameters, *a*, *b*, *c*, *d*, *f*, *g* and *h*

from subsection 1.1 are not constant, but they differ according to the applied production process. To model this relationship, the serial hybrid multilayer perceptron (SHMP) neural network according to Agarwal [19] was applied.

The multilayer perceptron (MP) is linked in series with the analytical model of the S-N curve and its scatter from Eqs. (3) and (4), see also Fig. 3 ([20]

and [21]). This means that the MP is applied first for
modelling the dependence of the parameters *a*, *b*, *c*,

*d*, *f*, *g* and *h* on the manufacturing technology and the
heat treatment. Then the analytical model is used only
for modelling the S-N curve and its scatter after the
seven parameters are predicted by the MP.

parameters of the applied production process. The *l*th
amplitude-stress level *Sa;l* is the independent variable
of the analytical model from subsection 1.1 and Fig. 3.
The *l*th_{ number-of-cycles-to-failure }_{N}_{l}_{ is the SHMP’s }
dependent variable and *n* is the total number of
sample points. Having this in mind, Eqs. (2) to (4) are
changed as follows:

*N N* *S* *f N* *N*

*N*
*a*

= →

### (

### )

= ⋅

⋅

⋅ −

−

( , ) ,

exp ,

**x** η β β

η η

η

β

β

1

(2)

η η η

η

= → = ⋅ +

+ ⋅

−

− +

( , ) ( ) ( , )

( ) ( , ) ,

( )

( ( ) ( ))

**x** **x** **x**

**x** **x**

**x**
**x** **x**

*S* *S* *a* *S*

*c* *S*

*a* *a* *a* *b*

*a* *b* *d* (9)

β β= =

= ⋅ +

+

### [

− ⋅ −### ]

( , )

( ) ( )

exp ( ) ( ( )) .

**x**

**x** **x**

**x** **x**

*S*

*f* *g*

*h* *S* *S*

*a*

*a* *KP*

1

1 (10)

The output of neuron *zj* is equal to the weighted
sum of *Mi* outputs *zi* from the preceding layer,
modified by an activation function *φj*:

*zj* *j* *w zij* *i*

*i*
*M*

*j*
*i*

= ⋅ +

=

### ∑

ϕ1

Θ , (11)

where* wij* are the synaptic weights and Q*j* is the
threshold of the neuron. In our case the activation
function was a tanh() function for the hidden neurons
and a linear function for the output neurons. This
activation function was used instead of the more
commonly used sigmoid function, because it turned
out that a convergence of a training process was

much better with the tanh() than with the sigmoid
function in the studied case. The inputs *xi* to the MP
model were the components of the condition vector **x**.
The output neurons *zk* are applied for calculating the
parameters *a*, *b*, *c*, *d*, *f*, *g* and *h*. The relations between
these parameters and the neural outputs *zk* must fulfill
the restraints from Eqs. (3) and (4) and ensure the
robustness of the model:

*a a* *z*

*z*
*ka*

*k*
*a*

= = ⋅

+

( ) exp( )

exp( ),

**x** 10000

1

*b b* *z*

*z*
*kb*

*kb*

= = + ⋅

+

( ) . . exp( )

exp( ),

**x** 0 01 0 99

1

*c c* *z*

*z*
*kc*

*kc*

= = ⋅

+

( ) exp( )

exp( ),

**x** 10
1

7

*d d* *z*

*z*
*k*
*d*

*k*
*d*

= = + ⋅

+

( ) . . exp( )

exp( ),

**x** 0 01 0 99

1

*f* *f* *z*

*z*
*kf*

*kf*

= = + ⋅

+

( ) exp( )

exp( ),

**x** 1 4
1

*g g* *z*

*z*
*kg*

*kg*

= = ⋅

+

( ) exp( )

exp( ),

**x** 3

1

*h h* *z*

*z*
*kh*

*kh*

= = ⋅

+

( ) . exp( )

exp( ).

**x** 0 1

1 (12)

These restraints were extensively tested in a preliminary study involving two different spring steels, a cold-drawn structural steel and two complex-phase steels.

The cost function for the SHMP model was
a maximum-likelihood function *EML* according to

Pascual and Meeker [22]. Using this cost function the
failed specimens as well as run-outs are considered
for estimating the S-N curve and its scatter. For the
fatigue failure a fatigue-failure identifier *δl* is set to
1 and for the run-outs it is set to 0 in the *EML* cost
function, see Eq. (13).

To calculate the error *eML*(*l*) for each sample

*l*, the parameters *a*, *b*, *c*, *d*, *f*, *g* and *h* are predicted
first by the MP for the input vector **x***i*. From these
parameters and the value of *Sa;l* the Weibull’s scale
parameter *ηpred;l* is calculated with Eq. (9) using the
Newton-Raphson method. The shape parameter *βpred;l*
is calculated with Eq. (10).

The training of the SHMP model was carried out
numerically with an error back-propagation algorithm
and an epoch-based training. The gradients of the cost
function *EML* for the synaptic weights *wij* were
calculated as the sum of the gradients of the individual
samples: ∂*E _{ML}*/∂

*w*=

_{ij}### ∑

_{l}n_{=}∂

*e l*( ) /∂

_{ML}*w*

_{ij}1 . In every

iteration of the training process the synaptic weights were adapted as follows [23]:

∆*w t* *t* *E* ∆

*w* *w t*

*ij* *ij* *ML*

*ij* _{t}*ij*

( ) ( ) ( ).

( )

= − + ⋅∂

∂ + ⋅ −

θ 1 α 1 (14)

The training process proceeds until the modelled
S-N curves with their scatter agree with the
experimental results for the different vectors **x***i*. The
training-rate parameter *θij* in Eq. (15) was added to
consider the past gradient changes according to the
delta-bar-delta rule [21].

The sample gradients ∂*eML*(*l*) / ∂*wij* were
calculated as follows ([21] and [22]):

∂*e lML*( ) ∂*wij*=∆*j*⋅*zi*, (15)

where D* _{j}* is the error of the neuron

*j*in the next layer to which the neuron

*i*sends its signal. The next layer of neurons is either a hidden or an output layer. To calculate the errors D

*in the output layer of the MP the partial derivatives ∂*

_{j}*eML*(

*l*) / ∂

*zk*for the output neurons

*zk* must be calculated for each sample (**x***l*, *Sa;l*, *Nl*, *δl*):

∂
∂ =
∂
∂ ⋅
∂
∂ +
∂
∂
*e l*
*z*
*e l*
*par*
*e l*
*ML*
*kpar*
*ML*
*pred l*

*pred l* *ML*
*pred l*
( ) ( ) ( )
,
,
,
η
η
β ⋅⋅
∂
∂ ⋅
∂
∂
⋅
⋅∂
∂ =
∂

β_{pred l}

*KP*
*KP*
*ka*
*S*
*S*
*par*
*par*

*z* *par a b c d*
*e*
,
; , , , ,
*M*
*ML*
*kpar*
*ML*
*pred l*
*pred l*
*kh*
*l*
*z*
*e l*
*par*
*par*

*z* *par f g*

( ) ( ) ; , , , ∂ = ∂ ∂ ⋅ ∂ ∂ ⋅ ∂ ∂ = β β

,, . (*h* 16)

For reasons of clarity, the marking of the
dependence on the vector **x** is omitted in Eq. (16) and
the corresponding partial derivatives are listed in the
appendix.

1.3 Selecting the Optimal SHMP Model

The SHMP model should represent the experimental
data {(**x***l*, *Sa;l*, *Nl*, *δl*); *l = *1, ..., *n*} in the best possible
way, but if the SHMP topology is too complex a
data over-fit can occur. So the complexity should
sometimes be sacrificed to avoid the over-fitting of
the SHMP model. In our study we decided to choose
the optimal topology of the SHMP model using the
Akaike information criterion (AIC) [23]:

*AIC*= ⋅2 *nw*+ ⋅2 ln(*EML*), (17)

where* nw* is the number of synaptic weights in the MP
and *EML* is the final value of the cost function. The
smaller the value of the AIC criterion, the better the
SHMP topology. In addition to the original form of the
AIC criterion, we also applied its modification with a
second-order correction for small samples [24]:

*AIC* *AIC* *n* *n*

*n n*

*c BA* *w* *w*
*w*
, = + .
⋅ ⋅

### (

### )

− − + 2 11 (18)

2 EXPERIMENTAL DATA

Cylindrical specimens according to the ASTM E 606-92 standard [25] were prepared by Institute of Metals

*E _{ML}*

_{= −}

*ML*

_{= −}

*f N*

_{l}

_{pred l}

_{pred l}*l*

*F N*

_{l}

_{pred l} ⋅ −

ln( ) ln ( |η _{,},β _{,}) δ 1 ( |η _{,},ββ

δ
δ
*pred l*
*l*
*n*
*ML* *ML*
*l*
*n*
*l* *l*
*l*

*E* *e l* *f N*

,) ,

( ) ln ( |

_{}
= = − ⋅
=
−
=

### ∏

### ∑

1 1 1ηη* _{pred l}*,,β

*,) ( δ*

_{pred l}*) ln*

_{l}*F N*(

*|η*

_{l}*,,β*

_{pred l}*,)*

_{pred l} + − ⋅1 _{}1− _{}

## {{

## }

= = − ⋅ ⋅ _{} ⋅ = −

### ∑

*l*

*n*

*l* *pred l*
*pred l*

*l*
*pred l*

*N* *pred l*

1 1 δ β η η β ln , , , , e

exp ( ) ln exp

,
,
−
_{}
+ − ⋅
*Nl*

*pred l* *l*
*pred l*

η δ

β

1 −−

_{}
=

### ∑

*Nl*

*pred l*
*l*

*n* *pred l*

η

β

,

,

1

and Technology. They were cut from 51CrV4 steel
bars in the rolling direction and manufactured by
turning. In the middle the specimens were polished to
an average roughness *Ra* of 0.2 mm, see Fig. 4. The
steel bars were produced by two manufacturing routes.
The reference series was prepared by a conventional
manufacturing technology, i.e. continuous casting
and hot rolling. The alternative series was first
continuously cast, then electro-slag remelted (ESR)
in order to obtain more uniform microstructure and
finally hot rolled.

Fig. 4. Cylindrical specimen used for the fatigue experiments
Cylindrical test specimens from both series were
subjected to two different heat treatment procedures.
The first heat treatment of the specimens consisted
of heating to 870 °C, soaking for 10 minutes, which
was followed by quenching in *N*2 gas at 5 bar and a
fast cooling rate of 7.5 °C/s until 60 °C. The second
heat treatment of the specimens was performed at the

same austenitizing temperature of 870 °C but a slower
cooling rate of 2.7 °C/s was obtained by reducing *N*2
gas pressure to 1.05 bar. In both cases the specimens
were finally tempered at 475 °C for 1 h.

Therefore four different groups of specimens were obtained: two different manufacturing technology routes combined with two different heat treatments. Altogether 101 specimens were manufactured with at least 23 specimens in each group [26].

The fatigue-life experiments were carried out
at the universal dynamic servo-hydraulic test stand
Instron 8802. A Dynacell load sensor was used
for force measurements and the experiments were
load-controlled. The axial loading of the cylindrical
specimens was fully reversed (*R* = –1). The
experiments were carried out at a room temperature
of 21 °C at different amplitude-stress levels (500
MPa to 780 MPa) until the fatigue failure occurred.
The testing frequency was 30 Hz. If the number of
loading cycles exceeded 1 million without the fatigue
failure the experiment run was terminated in order to
reduce the experimental time and cost, since it follows
from the literature that the fatigue failure between
1 million and 2 millions of loading cycles is highly
unlikely for these kind of high-strength steels [12].
The experimental results are presented in Fig. 5.

3 RESULTS AND DISCUSSION

3.1 Defining the SHMP Topologies and Pre-Processing the Data

There are two independent parameters that represent the input for the SHMP (a binary variable indicating

the manufacturing technology and a real-valued
variable indicating the cooling rate after the
warming-up phase), so the number of neurons in the SHMP
input layer was two. The seven parameters *a*, *b*, *c*, *d*,

*f*, *g* and *h* were predicted by the SHMP. Therefore,
there were seven neurons in the output layer of the
SHMP. All the SHMPs had one hidden layer and four
different topologies consisting of 2 (NN_1), 3 (NN_2),
6 (NN_3) or 9 (NN_4) neurons in the hidden layer.

The training set was composed of all the *n *=
101 samples in Fig. 5. Many training processes were
carried out with different initial values of the synaptic
weights and training-rate parameters. A number of
iterations were limited to 2,000,000 for each training
process. The details on the training processes are
listed in Table 1 for the best achieved cost functions.
Variations of the cost-functions *EML* during these
training processes are presented in Fig. 6.

Fig. 6. A cost-function history during the training process

3.2 Prediction Results

We can see from Table 1 that the NN_4 topology
with the largest number of neurons in the hidden
layer resulted in the lowest value of the *EML* cost
function that was achieved before 1 million of training
iterations with no further reduction in the
cost-function, see Fig. 6.

However, this result is misleading, because the NN_4 topology had almost as much synaptic weights as there was the number of training samples. That is why this topology may be improper, since it is prone to data over-fitting.

From the viewpoint of the *AIC* and *AICc,BA*
criteria, the best topology was NN_1, with two
neurons in the hidden layer. The good score in the
two *AIC* criteria was only due to its small number of
synaptic weights, because its cost function was the
highest. This implies that its fit of the S-N curves to
the experimental data is not the best – see Figs. 7 and
8 for a comparison of the modelled S-N curves.

To assess the prediction quality of the SHMP
models the S-N curves with their scatter were
additionally estimated on a case-by-case basis. The
seven parameters *a*, *b*, *c*, *d*, *f*, *g* and *h* for each of the
four S-N curves were estimated using the real-valued
genetic algorithm ([27] and [28]). The S-N curves,
which were estimated using the genetic algorithm, are
presented with a black color in Figs. 7 and 8.

It can be concluded from Table 1 and Figs. 7 and 8 that the best fit to the fatigue-life data is achieved with the NN_3 and NN_4 topologies. This

Table 1. *Summary of the applied SHMP topologies and their training processes*

SHMP topology NN_1 NN_2 NN_3 NN_4

Basic data about the SHMP topologies and their training processes

No. of input neurons 2 2 2 2

No. of output neurons 7 7 7 7

Act. function of output neurons linear linear linear linear

No. of hidden layers and neurons 1 layer, 2 neurons 1 layer, 3 neurons 1 layer, 6 neurons 1 layer, 9 neurons

Act. function of hidden neurons tanh() tanh() tanh() tanh()

Initial value of the parameter *η* 10–8 _{10}–8 _{10}–8 _{10}–8

Value of the parameter *α* 10–2 10–2 10–2 10–2

Initial (final) value of the param. *κ* 5×10–12 _{10}–11 _{10}–11 _{5×10}–12

Initial (final) value of the param. *γ* 0.995 0.99 0.99 0.995

Value of the parameter *ξ* 0.7 0.7 0.7 0.7

No. of train. Samples per epoch 101 101 101 101

Iteration no. for the minimum CF 2000000 2000000 2000000 786200

Cost function values and the AIC criteria values for the trained SHMP

Smallest value of the CF *E _{ML}* 901.53 901.39 897.41 896.71

Number of synaptic weights *n _{w}* 27 37 67 97

AIC criterion 955.5311 975.3921 1031.407 1090.708

*a) * * b) *

*c) * * d) *

Fig. 7. Modelled S-N curves for the SHMP topologies NN_1 and NN_2; a) Conv., FCR, b) Conv., SCR, c) ESR, FCR, d) ESR, FCR

a) b)

c) d)

means that the most appropriate topology was NN_3
with less neurons in the hidden layer, because the
discrepancy in the cost functions for the topologies
is almost insignificant. Due to the relatively small
number of training data the NN_3 topology has better
generalisation ability and is less prone to the
data-overfitting. Besides, it resulted in the lower values of
the two *AIC* and criteria when compared to the NN_4
topology.

By comparing the S-N curves modelled with the
SHMP and the genetic algorithm, it can be concluded
that the modelled S-N curves do not differ a lot for
the NN_3 and NN_4 topologies. This means that the
SHMP topologies NN_3 and NN_4 were successfully
applied for modelling the fatigue-life data of the
51CrV4 steel. The only exception is the S-N curve
model for the data set that corresponds to the ESR
manufacturing combined with the fast cooling rate
during quenching. In this case the transition zone
between the high-cycle- and very-high-cycle-fatigue
domains is very broad in both directions (*Sa* and *N*).
This is very difficult to model with a SHMP, given the
fact that the same transition zone is much narrower
for the other three data sets. For this reason it was
extremely difficult to build a good S-N curve model,
even if we try to do it individually with the genetic
algorithm.

From the presented results it can be concluded that the introduced SHMP model is capable of modelling the S-N curve and its scatter well, also in the neighbourhood of a knee point between the high-cycle- and very-high-cycle-fatigue domains. Of course, since there is always a problem with a relatively small number of experimental fatigue-life data one should always try to find the simplest possible SHMP model that still enables fairly good predictions of the S-N curves and their scatter. The applied SMHP is general, which means that it can be applied for modelling the S-N curves and their scatter for arbitrary (metallic) materials, if the appropriate experimental data are available and the fatigue-life data-sets have approximately equal size for different manufacturing technologies.

4 CONCLUSION

In this article a procedure is presented for predicting the S-N curves and their scatter for 51CrV4 spring steel on the basis of experimental fatigue-life data that was obtained for different manufacturing technologies and heat treatments. The procedure is based on the application of a multilayer perceptron neural network, into which an analytical shape of the bi-linear S-N

log-log curve was incorporated with the Weibull PDF describing its scatter. The results presented in the article were obtained for four combinations of the manufacturing technologies and quenching cooling rates. Different SHMP topologies were applied and each of them was trained with 101 experimentally obtained samples.

The results presented in the article show that it is possible to simultaneously estimate the parameters of the S-N curves and their scatter on the basis of the experimental data for different combinations of manufacturing technologies and heat treatments. The selection of a suitable SHMP topology should be made very carefully. It is almost always possible to obtain a good fit to the training data, if complex SHMP topologies with large numbers of neurons in the hidden layer are applied. On the other hand, such topologies can over-fit the data, especially if the number of synaptic weights in the SHMP model is comparable or larger than the number of data points in the training set. For this reason two variations of the AIC were applied in the research to select the proper SHMP topology. It turned out that the AIC criterion alone was not enough to estimate the most appropriate SHMP topology. So, when choosing the optimal SHMP model, one should make a trade-off between the simplicity of the SHMP model and its ability to generalise (but not over-fit) the experimental data. A general rule-of-thumb would be that there should be at least a few times more data points in the training set than there are synaptic weights in the SHMP model.

5 ACKNOWLEDGEMENT

The authors acknowledge the financial support from the Slovenian Research Agency (ARRS) for supporting the research programme P2-0182 R&D evaluations.

6 REFERENCES

[1] Nagode, M., Klemenc, J., Fajdiga, M. (2001). Parametric modelling and scatter prediction of rainflow matrices.

*International Journal of Fatigue*, vol. 23, no. 6, p. 525-532,

DOI:10.1016/S0142-1123(01)00007-X.

[2] Tovo, R. (2001). On the fatigue reliability evaluation of
structural components under service loading. *International *
*Journal of Fatigue*, vol. 23, no. 7, p. 587-598, DOI:10.1016/
S0142-1123(01)00021-4.

[4] O’Connor, P., Kleyner, A. (2012). *Practical Reliability *
*Engineering, 5th _{ ed}*

_{. John Willey & Sons, New York.}

[5] Xiao, Z., Zhao, Q.Y., Lin, F., Zhu, M.M., Deng, J.Y. (2018).
Studying the fatigue life of a non-pneumatic wheel by using
finite-life design for life prediction. *Strojniški vestnik - *
*Journal of Mechanical Engineering*, vol. 64, no. 1, p. 56-67,

DOI:10.5545/sv-jme.2017.4695.

[6] Moral Portalés R., Bochons Sania M.d.M., Klemenc, J.
(2018). Theoretical framework for estimating a product’s
reliability using a variable-amplitude loading spectrum and a
stress-based approach. *Fatigue and Fracture of Engineering *
*Materials and Structures*, vol. 41, no. 8, p. 1662-1673,

DOI:10.1111/ffe.12804.

[7] Gróza, M., Váradi, K. (2018). Fatigue design of ferritic-pearlitic nodular cast iron components with surface discontinuities.

*Strojniški vestnik - Journal of Mechanical Engineering*, vol. 64,
no. 6, p. 373-382, DOI:10.5545/sv-jme.2017.5120.

[8] Buxbaum, O. (1986). *Betriebsfestigkeit*. Verlag Stahleisen,
Düsseldorf.

[9] EUROCODE 3 (2005). *Design of Steel Structures – Part 1-9: *
*Fatigue*. European committee for standardization, Brussels.

[10] Bathias, C. (1999). There is no infinite fatigue life in metallic
materials. *Fatigue & Fracture of Engineering Materials & *
*Structures*, vol. 22, no. 7, p. 559-565,
DOI:10.1046/j.1460-2695.1999.00183.x.

[11] Haibach, E. (2006). *Betriebsfestigkeit, Verfahren und Daten *
*zur Bauteilberechnung. 3. Auflage*. Springer-Verlag, Berlin
Heidelberg.

[12] Toplack, G., Eichlseder, W., Godor, I., Leitner, H. (2003).
Influence of size and type of loading on S/N-Curve. *ESIS - *
*Cumulative Fatigue Damage Conference Proceedings*, p.
187-191.

[13] Schaumann, P., Steppler, S. (2013). Fatigue tests of axially

loaded butt welds up to very high cycles. *Procedia Engineering*,

vol. 66, p. 88-97, DOI:10.1016/j.proeng.2013.12.065.

[14] Wagener, R., Hensel, J. (2014). Einflussgrößen auf
die Lage des Abknickpunktes der Wöhlerlinie für den
Schwingfestigkeitsnachweis von Schweiß verbindungen (IGF
16602N), from *https://www.dvsev.de/fv/neu/indexcfm?Nav*
*igation=Forschungsergebnisse&PID=783&CFID=70346917*
*&CFTOKEN=97080438*, accessed on 2018-26-10.

Result score too low

[15] Dowling, N.E. (2012). *Mechanical Behaviour of Materials, *
*4th _{ ed. }*

_{Pearson Education, Upper Saddle River.}

[16] Klemenc, J., Fajdiga, M. (2013). Joint estimation of E-N curves
and their scatter using evolutionary algorithms. *International *
*Journal of Fatigue*, vol. 56, p. 42-53, DOI:10.1016/j.
ijfatigue.2013.08.005.

[17] Bučar, T., Nagode, M., Fajdiga, M. (2006). A neural network
approach to describing the scatter of S-N curves. *International *
*Journal of Fatigue*, vol. 28, no. 4, p. 311-323, DOI:10.1016/j.
ijfatigue.2005.08.002.

[18] Klemenc, J., Janezic, M., Fajdiga, M. (2012). Modelling the scatter of E-N curves using a serial hybrid neural network.

*Neural Computing and Applications*, vol. 21, no. 7, p.
1517-1530, DOI:10.1007/s00521-012-0828-2.

[19] Agarwal, M. (1997). Combining neural and conventional
paradigms for modelling, prediction and control. *International *
*Journal of System Science*, vol. 28, no. 1, p. 65-81.

[20] Bishop, C.M. (2005). *Neural Networks for Pattern Recognition*.

Clarendon Press, Oxford.

[21] Haykin, S. (2009). *Neural Networks and Learning Machines*.

Pearson education, New York.

[22] Pascual, F.G., Meeker, W.Q. (1999). Estimating fatigue curves
with the random fatigue-limit model. *Technometrics*, vol. 41,
no. 4, p. 277-290, DOI:10.2307/1271342.

[23] Akaike, H. (1974). A new look at the statistical model

identification. *IEEE Transactions on Automatic Control*, vol. 19,

no. 6, p. 716-723, DOI:10.1109/TAC.1974.1100705.

[24] Burnham, K.P., Anderson, D.R. (2002). Model Selection and Multimodel Inference: A Practical Information-Theoretic Approach, 2nd edition. Springer Verlag.

[25] ASTM E606-92(2004)e1: Standard Practice for
Strain-Controlled Fatigue Testing. *ASTM International*, West

Conshohocken, DOI:10.1520/E0606-92R04E01.

[26] Podgornik, B., Leskovšek, V., Godec, M., Senčič, B. (2014). Microstructure refinement and its effect on properties of

spring steel. *Materials Science & Engineering: A, Structural *

*Materials: Properties, Microstructure and Processing*, vol.

599, p. 81-86, DOI:10.1016/j.msea.2014.01.054.

[27] Temby, L., Vamplew, P., Berry A. (2005). Accelerating
real-valued genetic algorithms using
mutation-with-momentum. *The 18th _{ Australian Joint Conference on }*

*Artificial Intelligence*, vol 3809, Springer, Berlin, Heidelberg,

DOI:10.1007/11589990_149e.

[28] Klemenc, J. (2015). Influence of fatigue–life data modelling on the estimated reliability of a structure subjected to a constant-amplitude

loading. *Reliability Engineering and System Safety*, vol. 142, p. 238-247,

DOI:10.1016/j.ress.2015.05.026.
7 APPENDIX
∂
∂ = − ⋅ ⋅
_{}

*e l _{ML}*

*N*

*pred l* *l*
*pred l*
*pred l*
*l*
*pred l*
*pred*
( )
,
,
, ,
,
η δ
β
η η

β *ll* *pred*

*l* *pred l*
*pred l*
*l*
*pred l*
*N*
−
+ − ⋅ ⋅
_{}

1 (1 ) ,

, ,
,
δ β
η η
β *ll*

, (A.1)

∂_{∂} = − ⋅ +

_{}⋅ −

*e l _{ML}*

*N*

*N*

*pred l* *l* *pred l*

*l*
*pred l*
*l*
*pred*
( )
ln
, , ,
β δ β η η
1
1
,, ,
,

( ) ln

*l* *l*
*l*
*pred l*
*pred l*
*N*
− − ⋅
β
δ
η
1
⋅
*N _{l}*

*pred l*

*pred l*η β , ,

∂

∂ = − ⋅ ⋅ ⋅

⋅ −

+ _{} ⋅ −

β_{pred l}

*KP*

*a l* *KP*
*a l* *KP*

*S* *f g h*

*h S* *S*
*h S* *S*

, ,

,

exp ( )

exp ( )

1

## {

## }

2, (A.3)∂

∂ = ⋅ ⋅ − + ⋅ + ⋅ − −

η

η η

*pred l*

*pred l* *pred ld*

*a* *a b* *c b d*

,

, ( ) ,

, 1

1 1 (A.4)

∂
∂ = ⋅
∂
∂ = ⋅ ⋅ +
*S*
*a* *S*
*S*

*a* *S* *a*

*b*
*d*
*KP*

*KP* *KP* *KP*

ln( )

, 1

1 (A.5)

∂
∂ = +
*a*
*z*
*a*
*z*

*ka* 1 exp( *ka*)

, (A.6)

∂ ∂ = − ⋅ ⋅ ⋅ − − + ⋅ + ⋅ η η η η

*pred l* *a l* *pred l*
*pred lb* *pred*

*b*

*S*

*a b* *c b d*

, , ,
, ,
ln( )
( )
1
*ll*
*b d*

− − −1, (A.7)

∂
∂ = ⋅
∂
∂ = ⋅
−
*S*
*b* *S*
*S*
*b* *S*
*a* *c*
*d*
*KP*

*KP* *KP* *KP*

ln( ) ln( ) ln( )

, (A.8)

∂
∂ =
−
+
*b*
*z*
*b*
*z*

*kb* *kb*

0 01 1

.

exp( ), (A.9)

∂
∂ = ⋅ ⋅ − + ⋅ + ⋅ −
η
η η
*pred l*
*pred l*
*d*
*pred l*

*c* *a b* *c b d*

,

, ( ) ,

, 1

1 1 (A.10)

∂
∂ = ⋅
∂
∂ = ⋅
−
⋅
*S*
*c* *S*
*S*
*c* *S*
*b*
*c d*
*KP*

*KP* *KP* *KP*

ln( )

, (A.11)

∂
∂ = +
*c*
*z*
*c*
*z*

*kc* 1 exp( *kc*)

, (A.12)

∂ ∂ = − ⋅ ⋅ ⋅ − + ⋅ + ⋅ − η η η η

*pred l* *pred l*
*pred l*

*d*

*pred l*

*d*

*c*

*a b* *c b d*

, ,

, ,

ln( )

( ) ,

1 1 (A.13)

∂
∂ = ⋅
∂
∂ =
= ⋅−
_{}⋅

### [

−### ]

*S*

*d*

*S*

*S*

*d*

*S*

*b*

*d* *a* *c*

*KP*

*KP* *KP*

*KP*

ln( )

ln( ) ln( ) ,

2 (A.14)

∂
∂ =
−
+
*d*
*z*
*d*
*z*

*kd* *kd*

0 01 1

.

exp( ), (A.15)

∂

∂ = + + _{}− ⋅ − _{}

β_{pred l}

*a l* *KP*

*f*

*g*
*h S* *S*
,

,

exp ( ) ,

1

1 (A.16)

∂
∂ =
−
+
*f*
*z*
*f*
*z*

*kf* *kf*

1

1 exp( ), (A.17)

∂

∂ = + _{}− ⋅ − _{}

β_{pred l}

*a l* *KP*

*g*

*f*
*h S* *S*
,

,

exp ( ) ,

1 (A.18)

∂
∂ = +
*g*
*z*
*g*
*z*

*kg* 1 exp( *kg*)

, (A.19)

∂

∂ = ⋅ ⋅ − ⋅

⋅ ⋅ −

+ ⋅

β_{pred l}

*a l* *KP*
*a l* *KP*

*a l*

*h* *f g S* *S*

*h S* *S*
*h S*
,
,
,
,
( )

exp ( )

exp (

1 −−

## {

*S*)

_{KP}## }

,

2 (A.20)

∂
∂ = +
*h*
*z*
*h*
*z*

*kh* 1 exp( *kh*)